# Statistical evaluation of strain-life fatigue crack ...· 1 Statistical evaluation of strain-life

date post

30-Jul-2018Category

## Documents

view

218download

0

Embed Size (px)

### Transcript of Statistical evaluation of strain-life fatigue crack ...· 1 Statistical evaluation of strain-life

1

Statistical evaluation of strain-life fatigue crack initiation predictions

M.A. Meggiolaro *, J.T.P. Castro

Mechanical Engineering Department, Pontifical Catholic University of Rio de Janeiro (PUC-Rio)Rua Marqus de So Vicente 225, Rio de Janeiro, RJ, 22453-900, Brazil

Abstract

Most of the existing methods for estimating N parameters are based on a relatively limited

amount of experimental data. In addition, sound statistical evaluation of the popular rules of thumb

used in practice to estimate fatigue properties are scarce, if available. In this work, an extensive

statistical evaluation of the existing Coffin-Manson parameter estimates is presented based on

monotonic tensile and uniaxial fatigue properties of 845 different metals, including 724 steels, 81

aluminum alloys, and 15 titanium alloys. The studied Coffin-Manson estimates include the methods

proposed by Muralidharan and Manson, Bumel and Seeger, Roessle and Fatemi, Mitchell, Ong,

Morrow, Raske, as well as Manson's universal slopes and four-point correlation methods. From the

collected data it is shown that all correlations between the fatigue ductility coefficient f and the

monotonic tensile properties are very poor, and that it is statistically sounder to estimate f based

on constant values for each alloy family. Based on this result, a new estimation method which uses

the medians of the individual parameters of the 845 materials is proposed.

Keywords: Low-cycle fatigue; Estimation methods; Strain-life estimates; Statistical evaluation

1. Introduction

The so-called N fatigue design method correlates the number of cycles N to initiate a fatigue

crack in any structure with the life of small specimens made of the same material and submitted to

the same strain history that loads the critical point (generally a notch root) in service. This method

does not recognize the presence of cracks, however it models macroscopic elastic-plastic events at

* Corresponding author. Tel.: +55-21-3114-1638; fax: +55-21-3114-1165. E-mail address: meggi@mec.puc-rio.br

2

the notch roots and uses the local strain range (a more robust parameter to describe plastic effects)

instead of the stress range to quantify them. Therefore, the N method must be used to model low

cycle fatigue problems, when the plastic strain range p at the critical point is of the same order or

larger than the elastic range e, but it can be applied to predict any crack initiation life.

The classical N method works with real (logarithmic) stresses and strains, uses a Ramberg-

Osgood description for the hysteresis loops, and considers the cyclic softening or hardening

of the material, but not its transient behavior from the monotonic curve [1-5]. Hence, a single

equation is used to describe all hysteresis loops

'n/pe

'KE

1

22222

+=

+

=

(1)

where E is the Youngs modulus, K is the hardening coefficient and n is the hardening exponent of

the cyclically stabilized curve. Values for the cyclic hardening exponent n are typically

between 0.05 and 0.3, while the monotonic hardening exponent n is more disperse, varying between

0 and 0.5 in most cases.

The relationship between the stress range at the critical point and its fatigue initiation life N

is usually given by the classical Coffin-Manson equation

( ) cfbfpe )N('NE'

22222

+=

+

= (2)

where f, f, b and c are the fatigue strength and ductility coefficients and exponents measured in

fully alternated tension-compression fatigue tests.

Assuming that Ramberg-Osgoods elastic and plastic strain ranges perfectly correlate with the

correspondent Coffin-Mansons ranges, then only four of the six material parameters {n, K, f,

f, b, c} would be independent. Thus, from Eqs. (1-2),

== 'nc'nfb

f )N(''K)N(' 222 c

b'n = ; 'nf

f

'

''K

= (3)

3

The Ramberg-Osgood and Coffin-Manson equations describe well the cyclic response of many

materials, however they are not physical laws. Instead, Eq. (3) must be regarded as a measure of the

coherence between those equations. Therefore, such theoretical estimates should not be used to

replace experiments. Whenever possible, all six material parameters should be independently

obtained from actual measurements.

However, for initial design studies it is desirable to estimate these six N parameters based

only on readily available monotonic tensile test data. The main estimation methods proposed in the

literature are discussed next.

2. Estimation methods of fatigue properties

Several estimates of Coffin-Mansons parameters have been proposed in the literature since

Morrow [6], who in 1964 correlated the b and c exponents of Coffin-Mansons equation with the

cyclic hardening exponent n, see Table 1.

Based on experimental results on 69 metals, Manson [7] proposed in 1965 two different

methods: the Universal Slopes method, in which b and c are assumed constant for all metals

(namely b = 0.12 and c = 0.6), and the Four-Point Correlation method, defined through estimates

of the elastic or the plastic strain ranges e/2 or p/2 at four different lives (namely N = 1/4, 10,

104 and 105 cycles). Both Mansons estimates make use of the ultimate strength SU and the

reduction in area RA.

Raske and Morrow [8] published in 1969 an estimate for the fatigue ductility coefficient f

from f, n, and the cyclic yielding strength SY.

Mitchell [9] proposed in 1979 that the exponent b (and not only f) is a function of SU,

estimated f directly from the true fracture ductility f, and assumed that Mansons slope c = 0.6

is only valid for ductile metals, while c = 0.5 should be more appropriate for strong alloys.

4

In 1988, Muralidharan and Manson [10] revisited the Universal Slopes idea, increasing both

Coffin-Mansons exponents to b = 0.09 and c = 0.56, and introducing the parameter SU/E to

estimate both coefficients f and f.

Two years later, Bumel and Seeger [11] were the first to recognize the importance of

separating the N estimates by alloy family, proposing different methods for low-alloy steels and

for aluminum (Al) and titanium (Ti) alloys in their Uniform Material laws. It was found that in

average both exponents b and c are significantly lower in Al or Ti alloys than in steels, which might

explain the low value of b proposed by Manson in 1965, who included in his analyses several alloy

families besides steels [7]. Bumel and Seeger were also the first to ignore any monotonic measure

of the material ductility (such as the reduction in area RA) when estimating the fatigue ductility

coefficient f.

In 1993, Ong [12] revisited Mansons Four-Point Correlation method and proposed a few

modifications to better fit the experimental data of 49 steels from the SAE J1099 Technical Report

on Fatigue Properties [13]. Once again, b and c were assumed to be functions of the ultimate

strength SU and the true fracture ductility f, while f was estimated in the same way as Mitchell

proposed in 1979.

Recently, Roessle and Fatemi [14] proposed the Hardness method, assuming the same constant

slopes as Muralidharan and Manson did, while estimating both Coffin-Mansons coefficients as a

function of the Brinnell hardness HB. It is no surprise that f can be estimated from the hardness

HB, since SU and HB present a very good correlation for steels: if SU is given in MPa and HB in

kg/mm2, SU is approximately 3.4HB with a (small) coefficient of variation V = 3.8%, from a study

on 1924 steels from the ViDa software database [15-16].

In the last decade, several works have been published evaluating the life prediction errors

associated with each of the estimation methods discussed above [14, 17-20]. In 1993, Ong [17]

evaluated Mansons and Mitchells original methods based on properties of 49 steels. He concluded

5

that Mitchells method resulted in overly non-conservative predictions, while Mansons Universal

Slopes and Four-Point methods, although giving better life estimates, were only able to obtain

satisfactory correlations for the fatigue strength coefficient f. One year later, Brennan [18]

compared all of Mansons methods and concluded that Muralidharan-Mansons revised Universal

Slopes [10] resulted in good predictions, however his analysis was based on only six steels.

Park and Song [19] evaluated all methods proposed until 1995 using published data on 138

materials. They found that both Mansons original methods are excessively conservative for long

life predictions, but slightly non-conservative for short lives. In contrast, Muralidharan-Mansons

method is slightly conservative at shorter lives, but is non-conservative at long lives, being selected

as the best overall estimation method together with Bumel-Seegers uniform material laws. Park

and Song also confirmed that Mitchells method leads to non-conservative predictions over the

entire life range.

Roessle and Fatemi [14] studied measured properties of 20 steels plus 49 steels from the SAE

J1099 Technical Report on Fatigue Properties [13], arriving at basically the same conclusions as

Park and Song did. In addition, no strong correlation was found between f and the true fracture

strength. They also found that using the true fracture ductility f to esti

Recommended

*View more*